A Flexible Fluorescent SCC-MOF for Switchable Molecule Identification and Temperature Display
Dong, Xi-Yan; Huang, Hui-Lin; Wang, Jia-Yin; Li, Hai-Yang; Zang, Shuang-Quan; Chemistry of Materials 30 (2018) 2160–; doi:10.1021/acs.chemmater.8b00611

data_4002901
_publ_section_title
;
 A Flexible Fluorescent SCC-MOF for Switchable Molecule Identification and
 Temperature Display
;
_journal_issue                   6
_journal_name_full               'Chemistry of Materials'
_journal_page_first              2160
_journal_paper_doi               10.1021/acs.chemmater.8b00611
_journal_volume                  30
_journal_year                    2018
_chemical_formula_moiety         'C60 H82 Ag10 F6 N4 O10 P2 S6, 8(C H Cl3)'
_chemical_formula_sum            'C68 H90 Ag10 Cl24 F6 N4 O10 P2 S6'
_chemical_formula_weight         3421.23
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_audit_creation_date             2017-08-15
_audit_creation_method
;
Olex2 1.2
(compiled 2016.11.07 svn.r3352 for OlexSys, GUI svn.r5261)
;
_cell_angle_alpha                68.2840(10)
_cell_angle_beta                 74.9670(10)
_cell_angle_gamma                89.9200(10)
_cell_formula_units_Z            1
_cell_length_a                   12.1668(2)
_cell_length_b                   14.4398(2)
_cell_length_c                   18.3395(3)
_cell_measurement_reflns_used    16213
_cell_measurement_temperature    190.00(10)
_cell_measurement_theta_max      72.4080
_cell_measurement_theta_min      3.3600
_cell_volume                     2874.78(8)
_computing_cell_refinement       'CrysAlisPro 1.171.39.28b (Rigaku OD, 2015)'
_computing_data_collection       'CrysAlisPro 1.171.39.28b (Rigaku OD, 2015)'
_computing_data_reduction        'CrysAlisPro 1.171.39.28b (Rigaku OD, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      190.00(10)
_diffrn_detector                 'CCD plate'
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.992
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  t~exp~   \w     \q     \k     \f   Frames
--------------------------------------------------------------------------
  1  \w     17.00  55.00   0.25    0.25    --   45.20  38.00 120.00  152
  2  \w     20.00  88.00   0.25    0.25    --   45.20  57.00   0.00  272
  3  \w      9.00 132.00   0.25    0.25    --   45.20  38.00-120.00  492
  4  \w     80.00 109.00   0.25    0.25    --   45.20  38.00 120.00  116
  5  \w     -7.00  81.00   0.25    0.25    --   45.20 -82.00 150.00  352
  6  \w     27.00 114.00   0.25    0.25    --   45.20  57.00 -60.00  348
  7  \w    110.00 188.00   0.25    0.30    --  100.80  15.00-180.00  312
  8  \w     55.00  88.00   0.25    0.30    --  100.80  15.00-180.00  132
  9  \w     11.00  74.00   0.25    0.30    --  100.80 -61.00 150.00  252
 10  \w     11.00 190.00   0.25    0.30    --  100.80 -15.00 120.00  716
 11  \w     15.00  44.00   0.25    0.30    --  100.80  15.00-180.00  116
 12  \w     11.00  55.00   0.25    0.30    --  100.80 -82.00  90.00  176
 13  \w     66.00 116.00   0.25    0.30    --  100.80 -82.00  90.00  200
 14  \w     21.00 116.00   0.25    0.30    --  100.80 -61.00 -30.00  380
 15  \w     14.00  39.00   0.25    0.30    --  100.80 -61.00  30.00  100
 16  \w     74.00 120.00   0.25    0.30    --  100.80 -82.00-150.00  184
 17  \w     86.00 113.00   0.25    0.30    --  100.80 -61.00  30.00  108
 18  \w     37.00 142.00   0.25    0.30    --  100.80 -82.00 150.00  420
 19  \w     31.00 147.00   0.25    0.30    --  100.80 -30.00-180.00  464
 20  \w     77.00 103.00   0.25    0.30    --  100.80 -61.00 150.00  104
 21  \w     11.00 143.00   0.25    0.30    --  100.80 -82.00 -30.00  528
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'XtaLAB AFC12 (RINC): Kappa single'
_diffrn_measurement_method       '\w scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      0.0496003000
_diffrn_orient_matrix_UB_12      -0.0767424000
_diffrn_orient_matrix_UB_13      0.0640138000
_diffrn_orient_matrix_UB_21      0.1003813000
_diffrn_orient_matrix_UB_22      0.0786038000
_diffrn_orient_matrix_UB_23      -0.0203340000
_diffrn_orient_matrix_UB_31      -0.0696114000
_diffrn_orient_matrix_UB_32      0.0356127000
_diffrn_orient_matrix_UB_33      0.0659744000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0595
_diffrn_reflns_av_unetI/netI     0.0624
_diffrn_reflns_Laue_measured_fraction_full 0.992
_diffrn_reflns_Laue_measured_fraction_max 0.992
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            24263
_diffrn_reflns_point_group_measured_fraction_full 0.992
_diffrn_reflns_point_group_measured_fraction_max 0.992
_diffrn_reflns_theta_full        65.000
_diffrn_reflns_theta_max         65.000
_diffrn_reflns_theta_min         2.700
_diffrn_source                   'fine-focus sealed X-ray tube'
_diffrn_source_type              'Enhance (Cu) X-ray Source'
_exptl_absorpt_coefficient_mu    20.253
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.11589
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.39.28b (Rigaku Oxford Diffraction, 2015)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    1.976
_exptl_crystal_description       block
_exptl_crystal_F_000             1664
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.19
_exptl_crystal_size_min          0.13
_refine_diff_density_max         3.014
_refine_diff_density_min         -1.792
_refine_diff_density_rms         0.248
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.043
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     580
_refine_ls_number_reflns         9695
_refine_ls_number_restraints     42
_refine_ls_restrained_S_all      1.045
_refine_ls_R_factor_all          0.0799
_refine_ls_R_factor_gt           0.0751
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1351P)^2^+20.7247P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2081
_refine_ls_wR_factor_ref         0.2122
_reflns_Friedel_coverage         0.000
_reflns_number_gt                8621
_reflns_number_total             9695
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            cm8b00611_si_005.cif
_cod_data_source_block           ag10bpy_chcl3_190k
_cod_depositor_comments
'Adding full bibliography for 4002893--4002902.cif.'
_cod_database_code               4002901
_chemical_oxdiff_formula         'C H O N S Ag'
_reflns_odcompleteness_completeness 99.07
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     66.97
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All C(H,H) groups
 At 1.5 times of:
  All C(H,H,H) groups, All O(H) groups
2. Restrained distances
 Cl3-C34
 1.78 with sigma of 0.01
 Cl2B-Cl3B \\sim Cl3B-Cl1B \\sim Cl1B-Cl2B
 with sigma of 0.01
 Cl2-C34 \\sim Cl3-C34 \\sim Cl1-C34
 with sigma of 0.01
 Cl3B-C34B \\sim Cl2B-C34B \\sim Cl1B-C34B \\sim Cl3-C34 \\sim Cl1-C34 \\sim
Cl2-C34
 with sigma of 0.01
 Cl5B-Cl6B \\sim Cl6B-Cl4
 with sigma of 0.01
 Cl5-C33 \\sim Cl5B-C33 \\sim Cl6-C33 \\sim Cl6B-C33 \\sim Cl4-C33
 with sigma of 0.01
3. Uiso/Uaniso restraints and constraints
C34 \\sim C34B: within 2A with sigma of 0.01 and sigma for terminal atoms of
0.02
Cl2 \\sim Cl1 \\sim Cl3 \\sim Cl2B \\sim Cl1B \\sim Cl3B: within 2A with sigma
of 0.01 and sigma for terminal atoms of 0.02
Cl4 \\sim Cl6B \\sim Cl5B \\sim Cl6 \\sim Cl5: within 2A with sigma of 0.01 and
sigma for terminal atoms of 0.02
Uanis(C10) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
4. Others
 Fixed Sof: Cl6(0.5) Cl6B(0.5) Cl5(0.5) Cl5B(0.5) H33A(0.5) H33(0.5) Cl1(0.5)
 Cl2(0.5) Cl3(0.5) C34(0.5) H34(0.5) Cl2B(0.5) Cl1B(0.5) Cl3B(0.5) C34B(0.5)
 H34B(0.5)
5.a Ternary CH refined with riding coordinates:
 C33(H33A), C33(H33), C34(H34), C31(H31), C34B(H34B), C32(H32)
5.b Aromatic/amide H refined with riding coordinates:
 C17(H17), C16(H16), C14(H14), C13(H13), C22(H22), C21(H21), C19(H19),
 C18(H18), C24(H24), C25(H25), C26(H26), C27(H27), C28(H28)
5.c Idealised Me refined as rotating group:
 C4(H4A,H4B,H4C), C2(H2A,H2B,H2C), C3(H3A,H3B,H3C), C7(H7A,H7B,H7C), C6(H6A,
 H6B,H6C), C8(H8A,H8B,H8C), C12(H12A,H12B,H12C), C11(H11A,H11B,H11C), C10(H10A,
 H10B,H10C)
5.d Idealised tetrahedral OH refined as rotating group:
 O5(H5)
comments: The C11 in terminal t-butyl mercaptan group was slightly 
disordered. Its ADP was restrained with "ISOR" command. Four CHCl3 
molecules were assigned from a difference Fourier map. 
Two of them could be located easily due to the strong hydrogen bond and 
lone pair electrons interaction with the host framework, and refined 
anisotropically. The other two are highly disordered in the cavity. 
The disordered models obtained by splitting each CHCl3 over two sites 
with fixed occupancy ratio of 0.75:0.25 and 0.5:0.5, respectively. 
The disordered CHCl3 molecules were kept isotropic, and restrained 
using "SADI" and "SIMU" commands.
;
_shelx_shelxl_version_number     2016/6
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 3.441
_oxdiff_exptl_absorpt_empirical_full_min 0.395